Flux Synthesis, Structure, Properties, and Theoretical Magnetic Study of Uranium(IV)-Containing A2USi6O15 (A = K, Rb) with an Intriguing Green-to-Purple, Crystal-to-Crystal Structural Transition in the K Analogue.
Morrison, Gregory; Ramanantoanina, Harry; Urland, Werner; Smith, Mark D.; Zur Loye, Hans-Conrad; Inorganic chemistry 54 (2015) 5504–5511; doi:10.1021/acs.inorgchem.5b00556

data_4342856
_publ_section_title
;
 Flux Synthesis, Structure, Properties, and Theoretical Magnetic Study of
 Uranium(IV)-Containing A2USi6O15 (A = K, Rb) with an Intriguing
 Green-to-Purple, Crystal-to-Crystal Structural Transition in the K
 Analogue.
;
_journal_issue                   11
_journal_name_full               'Inorganic chemistry'
_journal_page_first              5504
_journal_page_last               5511
_journal_paper_doi               10.1021/acs.inorgchem.5b00556
_journal_volume                  54
_journal_year                    2015
_chemical_formula_moiety         'K2 O15 Si6 U'
_chemical_formula_sum            'K2 O15 Si6 U'
_chemical_formula_weight         724.77
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_audit_creation_method           SHELXL-2014/6
_cell_angle_alpha                99.514(2)
_cell_angle_beta                 91.002(2)
_cell_angle_gamma                106.116(2)
_cell_formula_units_Z            4
_cell_length_a                   7.2196(5)
_cell_length_b                   12.0518(8)
_cell_length_c                   17.1967(12)
_cell_measurement_reflns_used    9676
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      37.454
_cell_measurement_theta_min      2.325
_cell_volume                     1414.52(17)
_computing_cell_refinement       'SAINT-Plus Version 6.45 (Bruker, 2001)'
_computing_data_collection       'SMART Version 5.631 (Bruker, 2001)'
_computing_data_reduction        'SAINT-Plus Version 6.45 (Bruker, 2001)'
_computing_molecular_graphics    various
_computing_publication_material  various
_computing_structure_refinement  'SHELXL-2014/6 (Sheldrick, 2014)'
_computing_structure_solution    'SHELXS97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 0.929
_diffrn_measurement_device_type  'Bruker SMART APEX CCD diffractometer'
_diffrn_measurement_method       'omega and phi scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0350
_diffrn_reflns_av_unetI/netI     0.0370
_diffrn_reflns_laue_measured_fraction_full 1.000
_diffrn_reflns_laue_measured_fraction_max 0.929
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_k_max       18
_diffrn_reflns_limit_k_min       -18
_diffrn_reflns_limit_l_max       27
_diffrn_reflns_limit_l_min       -27
_diffrn_reflns_number            43979
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 0.929
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         35.033
_diffrn_reflns_theta_min         1.203
_diffrn_source                   'sealed tube'
_exptl_absorpt_coefficient_mu    12.654
_exptl_absorpt_correction_T_max  1.0000
_exptl_absorpt_correction_T_min  0.6532
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS Version 2.05 (Bruker, 2001)'
_exptl_crystal_colour            'light purple'
_exptl_crystal_density_diffrn    3.403
_exptl_crystal_description       irregular
_exptl_crystal_F_000             1336
_exptl_crystal_size_max          0.120
_exptl_crystal_size_mid          0.100
_exptl_crystal_size_min          0.080
_refine_diff_density_max         2.894
_refine_diff_density_min         -1.233
_refine_diff_density_rms         0.247
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.047
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     433
_refine_ls_number_reflns         11604
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.047
_refine_ls_R_factor_all          0.0351
_refine_ls_R_factor_gt           0.0294
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0267P)^2^+2.8824P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0604
_refine_ls_wR_factor_ref         0.0624
_reflns_number_gt                10408
_reflns_number_total             11604
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            ic5b00556_si_004.cif
_cod_data_source_block           kusiolts
_cod_depositor_comments
'Adding full bibliography for 4342855--4342857.cif.'
_cod_database_code               4342856
_shelx_estimated_absorpt_t_min   0.312
_shelx_estimated_absorpt_t_max   0.431
_shelxl_version_number           2014/6
_shelx_res_checksum              59528
_shelx_hkl_checksum              74617